View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
call for papers, research paper publishing, where to publish research paper, journal publishing, how to publish research paper, Call For research paper, international journal, publishing a paper, IJEI, call for papers 2012,journal of science and technolog
1.
International Journal of Engineering InventionsISSN: 2278-7461, www.ijeijournal.comVolume 1, Issue 2 (September 2012) PP: 56-61 Comparison of Low Field Electron Transport Properties in Compounds of groups III-V Semiconductors by Solving Boltzmann Equation Using Iteration Model H. Arabshahi1, A. Pashaei2 and M. H .Tayarani3 1 Physics Department, Payame Noor University, P. O. Box 19395-4697, Tehran, Iran 23 Physics Department, Higher Education Khayyam, Mashhad, IranAbstract––Temperature and doping dependencies of electron mobility in InP, InAs,GaP and GaAs structures have beencalculated using an iterative technique. The following scattering mechanisms, i.e, impurity, polar optical phonon,acoustic phonon and piezoelectric are included in the calculation. The electron mobility decreases monotonically as thetemperature increase from 100 K to 500 K for each material which is depended to their band structures characteristics.The low temperature value of electron mobility increases significantly with increasing doping concentration. Theiterative results are in fair agreement with other recent calculations obtained using the relaxation-time approximationand experimental methods.Keywords–– Iterative technique; Ionized impurity scattering; Born approximation; electron mobility I. INTRODUCTION The problems of electron transport properties in semiconductors have been extensively investigated boththeoretically and experimentally for many years. Many numerical methods available in the literature (Monte Carlo method,Iterative method, variation method, Relaxation time approximation, or Mattiessens rule) have lead to approximate solutionsto the Boltzmann transport equation [1-2]. In this paper iterative method is used to calculate the electron mobility of InAs,GaAs, InP and Gap. Because of high mobility InP has become an attractive material for electronic devices of superiorperformance among the IIIphosphates semiconductors.Therefore study of the electron transport in group IIIphosphates isnecessary. GaP possesses an indirect band gap of 0.6 eV at room temperature whereas InP have a direct band gap about 1.8eV, respectively. InP and InAs offer the prospect of mobility comparable to GaAs and are increasingly being developed forthe construction of optical switches and optoelectronic devices. The low-field electron mobility is one of the most important parameters that determine the performance of a field-effect transistor. The purpose of the present paper is to calculate electron mobility for various temperatures and ionized-impurity concentrations. The formulation itself applies only to the central valley conduction band. We have also considerband nonparabolicity and the screening effects of free carriers on the scattering probabilities. All the relevant scatteringmechanisms, including polar optic phonons, deformation potential, piezoelectric, acoustic phonons, and ionized impurityscattering. The Boltzmann equation is solved iteratively for our purpose, jointly incorporating the effects of all the scatteringmechanisms [3-4].This paper is organized as follows. Details of the iteration model , the electron scattering mechanismwhich have been used and the electron mobility calculations are presented in section II and the results of iterativecalculations carried out on Inp,InAs,GaP,GaAs structures are interpreted in section III. II. MODEL DETAIL To calculate mobility, we have to solve the Boltzmann equation to get the modified probability distributionfunction under the action of a steady electric field. Here we have adopted the iterative technique for solving the Boltzmanntransport equation. Under the action of a steady field, the Boltzmann equation for the distribution function can be written as f eF f v. r f . k f ( ) coll (1) t tWhere (f / t ) coll represents the change of distribution function due to the electron scattering. In the steady-state andunder application of a uniform electric field the Boltzmann equation can be written aseF f . k f ( ) coll (2) tConsider electrons in an isotropic, non-parabolic conduction band whose equilibrium Fermi distribution function is f0(k) inthe absence of electric field. Note the equilibrium distribution f0(k) is isotropic in k space but is perturbed when an electricfield is applied. If the electric field is small, we can treat the change from the equilibrium distribution function as a 56
2.
Comparison of Low Field Electron Transport Properties in Compounds of groups…perturbation which is first order in the electric field. The distribution in the presence of a sufficiently small field can bewritten quite generally as f (k ) f 0 (k ) f1 (k ) cos (3)Where θ is the angle between k and F and f1(k) is an isotropic function of k, which is proportional to the magnitude of theelectric field. f(k) satisfies the Boltzmann equation 2 and it follows that:eF f0 t i 1 i 0 i 0 3 cos f S (1 f ) S f d k f S (1 f ) S f d k 1 i 0 i 0 3 (4)In general there will be both elastic and inelastic scattering processes. For example impurity scattering is elastic andacoustic and piezoelectric scattering are elastic to a good approximation at room temperature. However, polar and non-polar optical phonon scattering are inelastic. Labeling the elastic and inelastic scattering rates with subscripts el and inelrespectively and recognizing that, for any process i, seli(k’, k) = seli(k, k’) equation 4 can be written as eF f 0 f1cos [ Sinel (1 f 0 ) Sinel f 0 ] d 3k f1 (k ) k (5) (1 cos )Sel d 3k [Sinel (1 f0 ) Sinel f0] d 3k Note the first term in the denominator is simply the momentum relaxation rate for elastic scattering. Equation 5 may besolved iteratively by the relation eF f 0 f1cos [n 1][Sinel (1 f 0 ) Sinel f 0 ] d 3k f1n (k ) k (6) (1 cos )Sel d 3k [Sinel (1 f0 ) Sinel f0] d 3k Where f 1n (k) is the perturbation to the distribution function after the n-th iteration. It is interesting to note that if the initialdistribution is chosen to be the equilibrium distribution, for which f 1 (k) is equal to zero, we get the relaxation timeapproximation result after the first iteration. We have found that convergence can normally be achieved after only a fewiterations for small electric fields. Once f 1 (k) has been evaluated to the required accuracy, it is possible to calculatequantities such as the drift mobility which is given in terms of spherical coordinates by (k / 1 2 F ) f1 d 3 k 3 * 0 (7) 3m F k 2 3 f0d k 0 Here, we have calculated low field drift mobility in III-V structures using the iterative technique. In the followingsections electron-phonon and electron-impurity scattering mechanisms will be discussed.Deformation potential scattering The acoustic modes modulate the inter atomic spacing. Consequently, the position of the conduction and valenceband edges and the energy band gap will vary with position because of the sensitivity of the band structure to the latticespacing. The energy change of a band edge due to this mechanism is defined by a deformation potential and the resultantscattering of carriers is called deformation potential scattering. The energy range involved in the case of scattering byacoustic phonons is from zero to 2vk , where v is the velocity of sound, since momentum conservation restricts thechange of phonon wave vector to between zero and 2k, where k is the electron wave vector. Typically, the average value of kis of the order of 107 cm-1 and the velocity of sound in the medium is of the order of 10 5 cms-1. Hence, 2vk ~ 1 meV,which is small compared to the thermal energy at room temperature. Therefore, the deformation potential scattering byacoustic modes can be considered as an elastic process except at very low temperature. The deformation potential scatteringrate with either phonon emission or absorption for an electron of energy E in a non-parabolic band is given by Fermisgolden rule as [3,5] 2 D 2 ac (mt ml )1/ 2 K BT E (1 E ) *2 *Rde v 2 4 E (1 2E ) (8)(1 E ) 2 1 / 3(E ) 2 Where Dac is the acoustic deformation potential, is the material density and is the non-parabolicity coefficient. Theformula clearly shows that the acoustic scattering increases with temperaturePiezoelectric scattering The second type of electron scattering by acoustic modes occurs when the displacements of the atoms create anelectric field through the piezoelectric effect. The piezoelectric scattering rate for an electron of energy E in an isotropic,parabolic band has been discussed by Ridley [4] . 57
3.
Comparison of Low Field Electron Transport Properties in Compounds of groups…The expression for the scattering rate of an electron in a non-parabolic band structure retaining only the important terms canbe written as [3,5]: 2 e 2 K B TK av m*R PZ (k ) 1 2 1 2 2 2 s 2 21 3 ( ) 2 1 (9) Where s is the relative dielectric constant of the material and Kav is the dimensionless so called averageelectromechanical coupling constant.Polar optical phonon scattering The dipolar electric field arising from the opposite displacement of the negatively and positively charged atomsprovides a coupling between the electrons and the lattice which results in electron scattering. This type of scattering is calledpolar optical phonon scattering and at room temperature is generally the most important scattering mechanism for electronsin III-V .The scattering rate due to this process for an electron of energy E in an isotropic, non-parabolic band is [3-5] e2 2m* 1 1 1 2E RPO k PO 8 E (10) FPO E , EN op , N op 1 Where E = E±_wpo is the final state energy phonon absorption (upper case) and emission (lower case) and Nop isthe phonon occupation number and the upper and lower cases refer to absorption and emission, respectively. For smallelectric fields, the phonon population will be very close to equilibrium so that the average number of phonons is given by theBose- Einstein distribution.Impurity scattering This scattering process arises as a result of the presence of impurities in a semiconductor. The substitution of animpurity atom on a lattice site will perturb the periodic crystal potential and result in scattering of an electron. Since the massof the impurity greatly exceeds that of an electron and the impurity is bonded to neighboring atoms, this scattering is veryclose to being elastic. Ionized impurity scattering is dominant at low temperatures because, as the thermal velocity of theelectrons decreases, the effect of long-range Coulombic interactions on their motion is increased. The electron scattering byionized impurity centers has been discussed by Brooks Herring [6] who included the modification of the Coulomb potentialdue to free carrier screening. The screened Coulomb potential is written as e2 exp(q0r ) (11)V (r ) 4 0 s r Where s is the relative dielectric constant of the material and q0 is the inverse screening length, which under nodegenerate conditions is given by ne2 (12) q0 2 0 s K BT Where n is the electron density. The scattering rate for an isotropic, nonparabolic band structure is given by [3,5] Ni e4 (1 2E ) b (13)Rim Ln(1 b) 3/ 2 1 b 32 2m s ( ( E )) * 2 8 m* ( E ) (14) b 2q0 2 Where Ni is the impurity concentration. III. RESULTS We have performed a series of low-field electron mobility calculations for GaP, InP, GaAs and InAs materials.Low-field motilities have been derived using iteration methode.The electron mobility is a function of temperature andelectron concentration . Figures 1 show the comparison the electron mobility depends on the Temperature at the different electronconcentration in bulk Gap,GaAs,InP and InAs materials. figures 1 show that electrons mobility at the definite temperature300 k for the InAs semiconductors is gained about 8117cm2v-1s-1 and for GaAs, InP, Gap about 4883,4702,760 cm2v-1s-1.also electrons mobility decrease quickly by temperature increasing from 200k to 500 k for all the different electronconcentrations because temperature increasing causes increase of phonons energy too. So it causes a strong interaction 58
4.
Comparison of Low Field Electron Transport Properties in Compounds of groups…between electrons and these phonons that its result is increase of electrons scattering rate and finally decrease of electronsmobility. Our calculation results show that the electron mobility InAs is more than 3other materials this increasing is becauseof small effective mass. 20000 16 -3 Donor electron density=10 ( cm ) InAs Electron drift mobility (cm2 / V-s) 15000 10000 GaAs 5000 InP GaP 0 200 250 300 350 400 450 500 Temperature (K) Fig 1. Changes the electron mobility Function in terms of temperature in bulk InAs, GaAs, InP and GaP at the electron concentration 1016 (cm-3). Figure 2 shows comparison the electron mobility of InAs, GaAs, InP and GaP at the different Temperature .Ourcalculation results show that the electron mobility InAs is more than GaAs,InP and GaP 10000 Temperature= 300 K 8000 Electron drift mobility (cm / V-s) 2 InAs 6000 4000 GaAs InP 2000 GaP 5.00E+017 1.00E+018 -3 Donor electron density ( cm ) Fig 2. Changes the electron mobility Function in terms of room temperature in bulk InAs, GaAs, InP and GaP at the different electron concentration. Figures 3 shows comparison the electron mobility depends on the electron concentration at the differentTemperature in bulk GaP and InP materials. Semiconductors mobility decrease by electrons concentrations increasingbecause electrons increasing causes increase of ionized impurity centers in crystals that it causes times more electrons underthe influence of the Coulomb potential of impurity centers located that its result is increase of electrons scattering rate andfinally decrease of electrons mobility 59
5.
Comparison of Low Field Electron Transport Properties in Compounds of groups… GaP:T=200 K 4000 GaP:T=300 K InP:T=200 K InP:T=300 K Electron drift mobility (cm / V-s) 3000 2 2000 1000 5.00E+017 1.00E+018 Temperature (K) Fig 3. Changes the electron mobility Function in terms of electron concentration in bulk InP and GaP at the different Temperature 20000 16 -3 InAs:Ionized impurity densiy =10 [cm ] 17 -3 InAs:Ionized impurity densiy =10 [cm ] 16 -3 GaAs:Ionized impurity densiy =10 [cm ] 17 -3 GaAs:Ionized impurity densiy =10 [cm ] Electron drift mobility (cm / V-s) 15000 2 10000 5000 200 250 300 350 400 Temperature (K) Fig 4. Changes the electron mobility Function in terms of temperature in bulk GaAs and InAs at the different electron concentration.Figures 4 shows comparison the electron mobility depends on temperature at the different electron concentration in bulkInAs and GaAs materials. .Our calculation results show that the electron mobility InAs is more than GaAS IV. CONCLUSION 1. InAs semiconductor having high mobility of GaAs,GaP and InP because the effective mass is small compared with all of them 2. The ionized impurity scattering in all the semiconductor InAs,GaAs,InP and GaP at all temperatures is an important factor in reducing the mobility. 60
6.
Comparison of Low Field Electron Transport Properties in Compounds of groups… REFERENCES1. Arabshahi H, Comparison of SiC and ZnO field effect transistors for high power applications ,Modern Phys. Lett. B, 23 (2009) 2533-2539.2. J. Fogarty, W. Kong and R. Solanki, Solid State Electronics 38 (1995) 653-659.3. Jacoboni C, Lugli P (1989). The Monte Carlo Method for semiconductor and Device Simulation, Springer-Verlag.4. Ridley BK (1997). Electrons and phonons in semiconductor multilayers,Cambridge University Press.5. Moglestue C (1993). Monte Carlo Simulation of Semiconductor Devices,Chapman and Hall.6. Chattopadhyay D, Queisser HJ (1981). Review of Modern Physics,53,part1. 61
Views
Actions
Embeds 0
Report content